| ||Format||Pages||Price|| |
|4||$38.00||  ADD TO CART|
|Hardcopy (shipping and handling)||4||$38.00||  ADD TO CART|
|Standard + Redline PDF Bundle||8||$45.60||  ADD TO CART|
This specification covers 8 and 9% nickel alloy steel plates for use in the water quenched and tempered condition intended for the fabrication of welded pressure vessels. The materials shall be available in two types, namely Type I and II, having different chemical compositions. The maximum thickness of plates is limited only by the capacity of the material to meet the specified mechanical property requirements. The material is susceptible to magnetization and the use of magnets in handling after heat treatment should be avoided if residual magnetism would be detrimental to subsequent fabrication or service. The steels shall be killed and shall conform to the fine austenitic grain size requirement specified. The plates shall be tempered and hardened by heat treatment. The specimens shall be subjected to tension and Charpy V-notch impact tests.
This abstract is a brief summary of the referenced standard. It is informational only and not an official part of the standard; the full text of the standard itself must be referred to for its use and application. ASTM does not give any warranty express or implied or make any representation that the contents of this abstract are accurate, complete or up to date.
1.1 This specification covers 7, 8, and 9 % nickel alloy steel plates for use in the water quenched and tempered condition intended for the fabrication of welded pressure vessels.
1.2 Material under this specification is available in three types having different chemical composition as follows:
Nominal Nickel Content, %
1.3 Plates produced under this specification are subject to impact testing at −320°F [−195°C] for Type I or Type III, and −275°F [−170°C] for Type II; or at such other temperatures as are agreed upon.
1.4 The maximum thickness of plates is limited only by the capacity of the material to meet the specified mechanical property requirements; however, current mill practice normally limits this material to 2 in. [50 mm] max.
1.5 This material is susceptible to magnetization. Use of magnets in handling after heat treatment should be avoided if residual magnetism would be detrimental to subsequent fabrication or service.
1.6 The values stated in either inch-pound units or SI units are to be regarded separately as standard. Within the text, the SI units are shown in brackets. The values stated in each system are not exact equivalents; therefore, each system must be used independently of the other. Combining values from the two systems may result in nonconformance with the specification.
1.7 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
A20/A20M Specification for General Requirements for Steel Plates for Pressure Vessels
A435/A435M Specification for Straight-Beam Ultrasonic Examination of Steel Plates
A577/A577M Specification for Ultrasonic Angle-Beam Examination of Steel Plates
ICS Number Code 77.140.50 (Flat steel products and semi-products)
UNSPSC Code 30102204(Steel plate )
ASTM A553 / A553M-14, Standard Specification for Pressure Vessel Plates, Alloy Steel, Quenched and Tempered 7, 8, and 9 % Nickel, ASTM International, West Conshohocken, PA, 2014, www.astm.orgBack to Top